#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/46/4504668.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4504668
loop_
_publ_author_name
'Wang, Jing-Ping'
'Zhao, Jun-Wei'
'Duan, Xian-Ying'
'Niu, Jing-Yang'
_publ_section_title
;
 Syntheses and Structures of One- and Two-Dimensional
 Organic−Inorganic Hybrid Rare Earth Derivatives Based on
 Monovacant Keggin-Type Polyoxotungstates
;
_journal_issue                   2
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              507
_journal_paper_doi               10.1021/cg050433j
_journal_volume                  6
_journal_year                    2006
_chemical_formula_sum            'C2 H39 O56.25 S Si Sm2.5 W11'
_chemical_formula_weight         3421.59
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 109.05(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   23.602(5)
_cell_length_b                   11.601(2)
_cell_length_c                   23.545(5)
_cell_measurement_reflns_used    250
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25
_cell_measurement_theta_min      2.5
_cell_volume                     6094(2)
_computing_cell_refinement       Raxis
_computing_data_collection       Raxis
_computing_data_reduction        Raxis
_computing_molecular_graphics    Texsan
_computing_publication_material  Texsan
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.907
_diffrn_measured_fraction_theta_max 0.907
_diffrn_measurement_device_type  R-axis-IV
_diffrn_measurement_method       'Osillation frames'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0992
_diffrn_reflns_av_sigmaI/netI    0.1037
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -28
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            15770
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.30
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    23.193
_exptl_absorpt_correction_T_max  0.2051
_exptl_absorpt_correction_T_min  0.1028
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    3.732
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Block
_exptl_crystal_F_000             6010
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.10
_refine_diff_density_max         3.542
_refine_diff_density_min         -3.280
_refine_diff_density_rms         0.468
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.974
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     784
_refine_ls_number_reflns         9742
_refine_ls_number_restraints     282
_refine_ls_restrained_S_all      0.964
_refine_ls_R_factor_all          0.0865
_refine_ls_R_factor_gt           0.0609
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0691P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1238
_refine_ls_wR_factor_ref         0.1322
_reflns_number_gt                7212
_reflns_number_total             9742
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg050433jsi20050822_015520.cif
_cod_data_source_block           njy1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from
2010-06-29.

'_exptl_absorpt_correction_type' value 'Empirical'
changed to 'empirical' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_H-M      P2(1)/c
_cod_original_formula_sum        'C2 H39 O56.25 S Si Sm2.50 W11'
_cod_database_code               4504668
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Sm1 Sm 0.22596(4) 0.50651(8) 0.32920(4) 0.0197(2) Uani 1 1 d .
Sm2 Sm 0.46210(5) 0.63145(9) 0.61219(5) 0.0270(2) Uani 1 1 d U
Sm3 Sm 0.0237(3) 1.4057(5) 0.0193(2) 0.0456(9) Uani 0.25 1 d PU
Sm4 Sm 0.0314(2) 1.0902(5) -0.0051(2) 0.0452(9) Uani 0.25 1 d PU
Si1 Si 0.2601(2) 0.8802(4) 0.3395(2) 0.0135(10) Uani 1 1 d .
W1 W 0.25193(4) 0.89278(7) 0.48519(3) 0.02246(19) Uani 1 1 d .
W2 W 0.13784(4) 0.76999(6) 0.37580(4) 0.02181(19) Uani 1 1 d .
W3 W 0.15812(4) 1.06213(7) 0.38165(4) 0.0245(2) Uani 1 1 d .
W4 W 0.16020(4) 1.05819(6) 0.22532(4) 0.02392(19) Uani 1 1 d .
W5 W 0.25469(4) 0.88108(6) 0.18875(3) 0.02088(19) Uani 1 1 d .
W6 W 0.13809(3) 0.76629(6) 0.22205(3) 0.02086(19) Uani 1 1 d .
W7 W 0.38276(3) 1.00198(6) 0.30831(4) 0.02002(18) Uani 1 1 d .
W8 W 0.38301(3) 1.00540(6) 0.45115(3) 0.01954(18) Uani 1 1 d .
W9 W 0.28971(3) 1.17913(6) 0.34748(3) 0.02016(19) Uani 1 1 d .
W10 W 0.35064(3) 0.68550(6) 0.44094(3) 0.01923(18) Uani 1 1 d .
W11 W 0.35344(3) 0.68178(6) 0.30283(3) 0.01961(18) Uani 1 1 d .
O1 O 0.2680(7) 0.8863(12) 0.5629(6) 0.035(4) Uani 1 1 d .
O2 O 0.0725(6) 0.7117(12) 0.3817(7) 0.038(4) Uani 1 1 d .
O3 O 0.1154(7) 1.1741(14) 0.3917(7) 0.043(4) Uani 1 1 d U
O4 O 0.1207(7) 1.1716(13) 0.1845(6) 0.037(4) Uani 1 1 d U
O5 O 0.2711(6) 0.8737(11) 0.1231(6) 0.030(3) Uani 1 1 d .
O6 O 0.0755(6) 0.7046(12) 0.1735(6) 0.034(3) Uani 1 1 d .
O7 O 0.4403(7) 1.0404(11) 0.2809(7) 0.035(4) Uani 1 1 d .
O8 O 0.4390(6) 1.0467(11) 0.5152(6) 0.029(3) Uani 1 1 d .
O9 O 0.2834(6) 0.3296(11) 0.3464(6) 0.033(3) Uani 1 1 d .
O10 O 0.4041(6) 0.6393(11) 0.5074(6) 0.024(3) Uani 1 1 d U
O11 O 0.4098(6) 0.6356(11) 0.2764(6) 0.030(3) Uani 1 1 d .
O12 O 0.4250(6) 1.0237(10) 0.3933(6) 0.025(3) Uani 1 1 d .
O13 O 0.2963(6) 0.7625(10) 0.4724(5) 0.020(3) Uani 1 1 d U
O14 O 0.1828(7) 0.6510(12) 0.3726(7) 0.037(4) Uani 1 1 d .
O15 O 0.3911(6) 0.8505(10) 0.4499(5) 0.021(3) Uani 1 1 d .
O16 O 0.3900(5) 0.8462(10) 0.3170(5) 0.019(3) Uani 1 1 d U
O17 O 0.1832(6) 0.7892(11) 0.1679(6) 0.031(3) Uani 1 1 d .
O18 O 0.1152(6) 0.7945(12) 0.2902(6) 0.033(3) Uani 1 1 d U
O19 O 0.3172(6) 0.9785(12) 0.2372(6) 0.031(3) Uani 1 1 d .
O20 O 0.2304(6) 1.1409(10) 0.3820(6) 0.026(3) Uani 1 1 d .
O21 O 0.3486(6) 1.1598(11) 0.4241(6) 0.028(3) Uani 1 1 d .
O22 O 0.3148(6) 0.9857(10) 0.4786(6) 0.021(3) Uani 1 1 d .
O23 O 0.1814(6) 0.7970(13) 0.4612(6) 0.032(3) Uani 1 1 d .
O24 O 0.3079(6) 0.5578(11) 0.2951(6) 0.026(3) Uani 1 1 d U
O25 O 0.1393(6) 1.0641(12) 0.2986(6) 0.032(3) Uani 1 1 d .
O26 O 0.1119(5) 0.9319(10) 0.1972(5) 0.017(3) Uani 1 1 d U
O27 O 0.3975(5) 0.6601(10) 0.3875(5) 0.020(3) Uani 1 1 d U
O28 O 0.3499(6) 1.1562(11) 0.3113(5) 0.025(3) Uani 1 1 d .
O29 O 0.1824(6) 0.6478(12) 0.2553(5) 0.027(3) Uani 1 1 d .
O30 O 0.2056(6) 1.0166(10) 0.1731(5) 0.018(3) Uani 1 1 d .
O31 O 0.2010(6) 1.0252(11) 0.4643(5) 0.022(3) Uani 1 1 d U
O32 O 0.3080(6) 0.5589(11) 0.4186(5) 0.022(3) Uani 1 1 d U
O33 O 0.2996(5) 0.7562(11) 0.2333(6) 0.025(3) Uani 1 1 d .
O34 O 0.2309(6) 1.1373(11) 0.2733(5) 0.022(3) Uani 1 1 d .
O35 O 0.1073(6) 0.9348(11) 0.3781(6) 0.029(3) Uani 1 1 d .
O36 O 0.3104(6) 0.9836(10) 0.3545(5) 0.018(3) Uani 1 1 d .
O37 O 0.2955(5) 0.7578(9) 0.3536(5) 0.015(3) Uani 1 1 d .
O38 O 0.2189(5) 0.8924(10) 0.2704(5) 0.016(3) Uani 1 1 d .
O39 O 0.2175(5) 0.8952(10) 0.3803(5) 0.018(3) Uani 1 1 d U
S1 S 0.0706(4) 0.4270(9) 0.2491(5) 0.065(2) Uani 0.80 1 d PU
S1' S 0.0683(16) 0.424(4) 0.3001(19) 0.065(2) Uani 0.20 1 d PU
O1A O 0.1262(7) 0.4390(14) 0.3020(8) 0.055(5) Uani 1 1 d .
C1 C 0.0187(12) 0.521(3) 0.2578(13) 0.065(2) Uani 1 1 d U
H1A H 0.0283 0.6025 0.2627 0.078 Uiso 1 1 calc R
H1B H -0.0235 0.5008 0.2423 0.078 Uiso 1 1 calc R
C2 C 0.0383(14) 0.303(3) 0.2602(15) 0.086(11) Uani 1 1 d .
H2A H 0.0615 0.2326 0.2674 0.103 Uiso 1 1 calc R
H2B H -0.0049 0.2955 0.2440 0.103 Uiso 1 1 calc R
O1W O 0.2090(7) 0.4008(13) 0.4153(8) 0.046(4) Uani 1 1 d .
O2W O 0.2071(8) 0.3996(13) 0.2317(6) 0.043(4) Uani 1 1 d .
O3W O 0.5703(6) 0.6249(12) 0.6404(6) 0.0301(13) Uani 1 1 d U
O4W O 0.3759(6) 0.5227(12) 0.6088(6) 0.0295(12) Uani 1 1 d U
O5W O 0.4870(6) 0.8107(12) 0.5698(6) 0.0288(11) Uani 1 1 d U
O6W O 0.4875(8) 0.4630(15) 0.5662(8) 0.056(5) Uani 1 1 d .
O7W O 0.4898(8) 0.4943(14) 0.6952(8) 0.050(4) Uani 1 1 d .
O8W O 0.3846(6) 0.7617(11) 0.6191(6) 0.0310(13) Uani 1 1 d U
O9W O 0.5012(6) 0.7464(12) 0.7035(6) 0.0330(13) Uani 1 1 d U
O10W O 0.3973(7) 1.3791(14) 0.4663(7) 0.044(4) Uani 1 1 d U
O11W O 0.5187(16) 0.820(4) 0.377(2) 0.078(13) Uani 0.50 1 d P
O12W O -0.6395(15) 2.113(2) -0.2639(13) 0.043(8) Uani 0.50 1 d P
O13W O 0.2883(15) 1.224(3) 0.1789(14) 0.047(8) Uani 0.50 1 d PU
O14W O 0.3715(12) 1.206(2) 0.1139(11) 0.024(6) Uani 0.50 1 d PU
O15W O -0.2153(18) 2.058(3) -0.0035(17) 0.065(10) Uani 0.50 1 d PU
O16W O 0.2772(11) 1.250(2) 0.5045(11) 0.023(6) Uani 0.50 1 d PU
O17W O -0.413(2) 2.482(4) -0.1492(19) 0.079(12) Uani 0.50 1 d PU
O18W O -0.127(2) 1.260(4) -0.044(2) 0.085(12) Uani 0.50 1 d PU
O19W O 0.020(3) 1.260(5) -0.074(3) 0.0455(10) Uani 0.25 1 d PU
O20W O 0.040(3) 0.944(6) 0.079(3) 0.0454(11) Uani 0.25 1 d PU
O21W O 0.098(3) 1.495(6) 0.113(3) 0.0462(15) Uani 0.25 1 d PU
O22W O 0.199(4) 1.249(7) 0.074(4) 0.08(2) Uani 0.25 1 d PU
O23W O -0.062(3) 1.439(6) 0.023(3) 0.0458(11) Uani 0.25 1 d PU
O24W O 0.096(3) 1.084(6) -0.069(3) 0.0457(15) Uani 0.25 1 d PU
O25W O 0.028(3) 1.289(6) 0.103(3) 0.0461(15) Uani 0.25 1 d PU
O26W O -0.026(3) 1.206(6) 0.019(3) 0.0455(10) Uani 0.25 1 d PU
O27W O 0.203(2) 1.551(4) 0.135(2) 0.025(11) Uani 0.25 1 d PU
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sm Sm -0.1638 3.4418 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O14 Sm1 O1A 79.6(6) . .
O14 Sm1 O29 71.4(4) . .
O1A Sm1 O29 82.8(5) . .
O14 Sm1 O24 118.5(5) . .
O1A Sm1 O24 146.4(6) . .
O29 Sm1 O24 77.7(4) . .
O14 Sm1 O9 145.8(5) . .
O1A Sm1 O9 102.6(5) . .
O29 Sm1 O9 142.7(4) . .
O24 Sm1 O9 78.3(5) . .
O14 Sm1 O32 77.4(5) . .
O1A Sm1 O32 139.5(5) . .
O29 Sm1 O32 119.8(4) . .
O24 Sm1 O32 74.1(4) . .
O9 Sm1 O32 79.7(5) . .
O14 Sm1 O1W 78.0(5) . .
O1A Sm1 O1W 69.5(6) . .
O29 Sm1 O1W 141.8(5) . .
O24 Sm1 O1W 138.6(5) . .
O9 Sm1 O1W 71.3(5) . .
O32 Sm1 O1W 73.4(5) . .
O14 Sm1 O2W 140.5(5) . .
O1A Sm1 O2W 74.1(6) . .
O29 Sm1 O2W 76.4(4) . .
O24 Sm1 O2W 74.9(5) . .
O9 Sm1 O2W 70.0(5) . .
O32 Sm1 O2W 140.2(5) . .
O1W Sm1 O2W 117.9(5) . .
O4W Sm2 O10 77.9(4) . .
O4W Sm2 O6W 83.7(6) . .
O10 Sm2 O6W 73.2(5) . .
O4W Sm2 O8W 71.1(5) . .
O10 Sm2 O8W 81.6(4) . .
O6W Sm2 O8W 147.5(5) . .
O4W Sm2 O3W 143.9(5) . .
O10 Sm2 O3W 118.7(4) . .
O6W Sm2 O3W 72.7(6) . .
O8W Sm2 O3W 139.0(5) . .
O4W Sm2 O7W 71.5(5) . .
O10 Sm2 O7W 139.7(5) . .
O6W Sm2 O7W 77.8(6) . .
O8W Sm2 O7W 111.4(5) . .
O3W Sm2 O7W 77.1(5) . .
O4W Sm2 O9W 113.2(5) . .
O10 Sm2 O9W 144.0(4) . .
O6W Sm2 O9W 139.7(5) . .
O8W Sm2 O9W 71.1(5) . .
O3W Sm2 O9W 73.3(5) . .
O7W Sm2 O9W 74.0(5) . .
O4W Sm2 O5W 138.7(5) . .
O10 Sm2 O5W 71.5(4) . .
O6W Sm2 O5W 112.1(5) . .
O8W Sm2 O5W 77.6(5) . .
O3W Sm2 O5W 76.6(4) . .
O7W Sm2 O5W 147.1(5) . .
O9W Sm2 O5W 79.9(4) . .
O23W Sm3 O25W 81(2) . .
O23W Sm3 O23W 112.9(18) . 3_585
O25W Sm3 O23W 150(2) . 3_585
O23W Sm3 Sm3 61.9(18) . 3_585
O25W Sm3 Sm3 134.2(16) . 3_585
O23W Sm3 Sm3 51.0(16) 3_585 3_585
O23W Sm3 O21W 107(2) . .
O25W Sm3 O21W 71(2) . .
O23W Sm3 O21W 79(2) 3_585 .
Sm3 Sm3 O21W 93.5(15) 3_585 .
O23W Sm3 O26W 74(2) . .
O25W Sm3 O26W 52(2) . .
O23W Sm3 O26W 155(2) 3_585 .
Sm3 Sm3 O26W 129.6(15) 3_585 .
O21W Sm3 O26W 123(2) . .
O23W Sm3 O19W 112(2) . .
O25W Sm3 O19W 107(2) . .
O23W Sm3 O19W 92(2) 3_585 .
Sm3 Sm3 O19W 110.8(14) 3_585 .
O21W Sm3 O19W 141(2) . .
O26W Sm3 O19W 63.7(19) . .
O23W Sm3 Sm4 106.5(18) . .
O25W Sm3 Sm4 65.1(16) . .
O23W Sm3 Sm4 129.4(15) 3_585 .
Sm3 Sm3 Sm4 147.9(3) 3_585 .
O21W Sm3 Sm4 118.6(15) . .
O26W Sm3 Sm4 33.4(14) . .
O19W Sm3 Sm4 42.5(13) . .
O20W Sm4 O26W 87(3) 3_575 .
O20W Sm4 O24W 89(2) 3_575 .
O26W Sm4 O24W 140(2) . .
O20W Sm4 O19W 74(2) 3_575 .
O26W Sm4 O19W 75(2) . .
O24W Sm4 O19W 65(2) . .
O20W Sm4 O20W 111.5(18) 3_575 .
O26W Sm4 O20W 96(2) . .
O24W Sm4 O20W 123(2) . .
O19W Sm4 O20W 169(2) . .
O20W Sm4 Sm4 65.6(18) 3_575 3_575
O26W Sm4 Sm4 93.0(18) . 3_575
O24W Sm4 Sm4 121.0(15) . 3_575
O19W Sm4 Sm4 138.0(15) . 3_575
O20W Sm4 Sm4 45.9(15) . 3_575
O20W Sm4 Sm3 105.1(19) 3_575 .
O26W Sm4 Sm3 42.6(18) . .
O24W Sm4 Sm3 101.1(15) . .
O19W Sm4 Sm3 47.8(14) . .
O20W Sm4 Sm3 121.6(14) . .
Sm4 Sm4 Sm3 135.6(3) 3_575 .
O38 Si1 O39 107.7(6) . .
O38 Si1 O37 112.6(6) . .
O39 Si1 O37 110.6(6) . .
O38 Si1 O36 108.0(6) . .
O39 Si1 O36 110.0(6) . .
O37 Si1 O36 107.9(6) . .
O1 W1 O22 101.7(6) . .
O1 W1 O31 102.0(6) . .
O22 W1 O31 88.0(5) . .
O1 W1 O13 100.8(6) . .
O22 W1 O13 87.3(5) . .
O31 W1 O13 157.2(5) . .
O1 W1 O23 98.9(6) . .
O22 W1 O23 159.4(5) . .
O31 W1 O23 88.7(6) . .
O13 W1 O23 87.8(6) . .
O1 W1 O39 172.4(6) . .
O22 W1 O39 85.3(5) . .
O31 W1 O39 75.3(5) . .
O13 W1 O39 82.1(5) . .
O23 W1 O39 74.2(5) . .
O2 W2 O14 105.3(7) . .
O2 W2 O18 101.0(7) . .
O14 W2 O18 92.0(6) . .
O2 W2 O23 99.4(7) . .
O14 W2 O23 92.7(7) . .
O18 W2 O23 157.0(6) . .
O2 W2 O35 91.8(6) . .
O14 W2 O35 162.9(6) . .
O18 W2 O35 84.8(6) . .
O23 W2 O35 84.0(6) . .
O2 W2 O39 163.4(6) . .
O14 W2 O39 90.1(6) . .
O18 W2 O39 84.3(5) . .
O23 W2 O39 73.2(5) . .
O35 W2 O39 72.9(5) . .
O3 W3 O25 100.8(7) . .
O3 W3 O35 101.9(7) . .
O25 W3 O35 91.8(6) . .
O3 W3 O31 99.7(6) . .
O25 W3 O31 158.8(6) . .
O35 W3 O31 89.3(6) . .
O3 W3 O20 101.5(6) . .
O25 W3 O20 84.6(6) . .
O35 W3 O20 156.6(5) . .
O31 W3 O20 85.9(5) . .
O3 W3 O39 172.3(6) . .
O25 W3 O39 86.3(5) . .
O35 W3 O39 74.5(5) . .
O31 W3 O39 73.6(5) . .
O20 W3 O39 82.1(5) . .
O4 W4 O26 104.4(6) . .
O4 W4 O34 99.9(6) . .
O26 W4 O34 155.6(5) . .
O4 W4 O30 98.5(6) . .
O26 W4 O30 88.8(5) . .
O34 W4 O30 86.4(5) . .
O4 W4 O25 102.8(7) . .
O26 W4 O25 92.4(5) . .
O34 W4 O25 83.4(5) . .
O30 W4 O25 157.7(6) . .
O4 W4 O38 172.2(5) . .
O26 W4 O38 73.9(5) . .
O34 W4 O38 81.8(5) . .
O30 W4 O38 73.9(4) . .
O25 W4 O38 85.0(5) . .
O5 W5 O33 102.2(6) . .
O5 W5 O19 102.1(6) . .
O33 W5 O19 86.5(6) . .
O5 W5 O30 99.7(5) . .
O33 W5 O30 157.9(5) . .
O19 W5 O30 86.0(5) . .
O5 W5 O17 100.4(6) . .
O33 W5 O17 90.2(6) . .
O19 W5 O17 157.4(6) . .
O30 W5 O17 88.9(5) . .
O5 W5 O38 172.4(6) . .
O33 W5 O38 82.8(5) . .
O19 W5 O38 83.8(5) . .
O30 W5 O38 75.8(4) . .
O17 W5 O38 73.7(5) . .
O6 W6 O29 103.4(7) . .
O6 W6 O18 102.6(6) . .
O29 W6 O18 92.9(6) . .
O6 W6 O17 99.1(6) . .
O29 W6 O17 91.5(5) . .
O18 W6 O17 156.2(6) . .
O6 W6 O26 95.0(6) . .
O29 W6 O26 161.3(5) . .
O18 W6 O26 86.4(5) . .
O17 W6 O26 82.0(5) . .
O6 W6 O38 164.7(5) . .
O29 W6 O38 90.0(5) . .
O18 W6 O38 83.9(5) . .
O17 W6 O38 72.7(5) . .
O26 W6 O38 71.3(4) . .
O7 W7 O16 103.9(6) . .
O7 W7 O19 102.7(7) . .
O16 W7 O19 88.6(6) . .
O7 W7 O12 98.5(6) . .
O16 W7 O12 90.9(5) . .
O19 W7 O12 158.2(6) . .
O7 W7 O28 98.4(6) . .
O16 W7 O28 157.7(5) . .
O19 W7 O28 86.8(5) . .
O12 W7 O28 85.5(5) . .
O7 W7 O36 169.2(5) . .
O16 W7 O36 84.9(5) . .
O19 W7 O36 83.5(5) . .
O12 W7 O36 74.8(5) . .
O28 W7 O36 72.9(5) . .
O8 W8 O15 103.7(6) . .
O8 W8 O22 103.0(6) . .
O15 W8 O22 89.5(5) . .
O8 W8 O12 99.4(6) . .
O15 W8 O12 91.0(5) . .
O22 W8 O12 156.8(5) . .
O8 W8 O21 98.4(6) . .
O15 W8 O21 157.9(5) . .
O22 W8 O21 85.2(5) . .
O12 W8 O21 85.8(5) . .
O8 W8 O36 168.4(6) . .
O15 W8 O36 85.7(5) . .
O22 W8 O36 83.6(5) . .
O12 W8 O36 73.3(5) . .
O21 W8 O36 72.4(5) . .
O9 W9 O20 99.7(6) 1_565 .
O9 W9 O28 101.9(6) 1_565 .
O20 W9 O28 158.3(5) . .
O9 W9 O21 99.4(6) 1_565 .
O20 W9 O21 88.8(6) . .
O28 W9 O21 89.3(5) . .
O9 W9 O34 102.0(6) 1_565 .
O20 W9 O34 85.1(6) . .
O28 W9 O34 88.9(5) . .
O21 W9 O34 158.4(5) . .
O9 W9 O36 173.0(6) 1_565 .
O20 W9 O36 84.7(5) . .
O28 W9 O36 73.9(5) . .
O21 W9 O36 75.2(5) . .
O34 W9 O36 83.7(5) . .
O10 W10 O32 100.8(6) . .
O10 W10 O13 100.2(5) . .
O32 W10 O13 96.6(6) . .
O10 W10 O27 97.9(5) . .
O32 W10 O27 94.0(5) . .
O13 W10 O27 156.9(5) . .
O10 W10 O15 91.0(5) . .
O32 W10 O15 168.1(5) . .
O13 W10 O15 82.9(5) . .
O27 W10 O15 82.5(5) . .
O10 W10 O37 170.6(5) . .
O32 W10 O37 86.2(5) . .
O13 W10 O37 85.2(5) . .
O27 W10 O37 75.1(5) . .
O15 W10 O37 81.9(4) . .
O11 W11 O24 103.0(6) . .
O11 W11 O33 101.9(6) . .
O24 W11 O33 93.9(6) . .
O11 W11 O27 96.4(6) . .
O24 W11 O27 96.0(5) . .
O33 W11 O27 156.7(5) . .
O11 W11 O16 90.8(5) . .
O24 W11 O16 166.1(5) . .
O33 W11 O16 81.3(5) . .
O27 W11 O16 84.2(5) . .
O11 W11 O37 168.0(6) . .
O24 W11 O37 85.4(5) . .
O33 W11 O37 85.9(5) . .
O27 W11 O37 73.9(5) . .
O16 W11 O37 81.3(4) . .
W9 O9 Sm1 152.6(8) 1_545 .
W10 O10 Sm2 159.6(7) . .
W7 O12 W8 120.1(7) . .
W10 O13 W1 154.7(7) . .
W2 O14 Sm1 158.2(8) . .
W8 O15 W10 148.6(7) . .
W7 O16 W11 151.1(7) . .
W5 O17 W6 122.4(7) . .
W6 O18 W2 143.7(8) . .
W7 O19 W5 149.5(8) . .
W9 O20 W3 152.5(7) . .
W9 O21 W8 120.5(7) . .
W1 O22 W8 149.3(7) . .
W1 O23 W2 120.5(7) . .
W11 O24 Sm1 134.2(7) . .
W3 O25 W4 152.9(9) . .
W4 O26 W6 123.4(6) . .
W11 O27 W10 114.6(6) . .
W9 O28 W7 120.5(6) . .
W6 O29 Sm1 157.8(6) . .
W5 O30 W4 120.5(6) . .
W1 O31 W3 121.1(6) . .
W10 O32 Sm1 133.1(6) . .
W5 O33 W11 155.6(7) . .
W9 O34 W4 153.6(7) . .
W3 O35 W2 120.5(7) . .
Si1 O36 W7 124.0(6) . .
Si1 O36 W9 125.4(7) . .
W7 O36 W9 92.7(4) . .
Si1 O36 W8 121.9(6) . .
W7 O36 W8 91.6(4) . .
W9 O36 W8 91.9(4) . .
Si1 O37 W10 129.0(6) . .
Si1 O37 W11 126.1(6) . .
W10 O37 W11 94.0(4) . .
Si1 O38 W5 124.4(6) . .
Si1 O38 W6 123.8(6) . .
W5 O38 W6 91.1(4) . .
Si1 O38 W4 126.1(6) . .
W5 O38 W4 89.6(4) . .
W6 O38 W4 91.4(4) . .
Si1 O39 W1 124.0(7) . .
Si1 O39 W2 123.5(6) . .
W1 O39 W2 92.2(4) . .
Si1 O39 W3 125.2(6) . .
W1 O39 W3 90.0(4) . .
W2 O39 W3 92.2(4) . .
S1' S1 O1A 59.3(18) . .
S1' S1 C2 70(2) . .
O1A S1 C2 105.5(14) . .
S1' S1 C1 69(2) . .
O1A S1 C1 108.1(13) . .
C2 S1 C1 98.4(17) . .
S1 S1' O1A 70(2) . .
S1 S1' C1 69(2) . .
O1A S1' C1 115(3) . .
S1 S1' C2 68(2) . .
O1A S1' C2 111(3) . .
C1 S1' C2 98(2) . .
S1' O1A S1 50.3(18) . .
S1' O1A Sm1 162(2) . .
S1 O1A Sm1 141.6(12) . .
S1' C1 S1 42.1(16) . .
S1' C1 H1A 119.3 . .
S1 C1 H1A 119.3 . .
S1' C1 H1B 119.3 . .
S1 C1 H1B 119.3 . .
H1A C1 H1B 116.8 . .
S1 C2 S1' 42.2(17) . .
S1 C2 H2A 119.3 . .
S1' C2 H2A 119.3 . .
S1 C2 H2B 119.3 . .
S1' C2 H2B 119.3 . .
H2A C2 H2B 116.8 . .
Sm4 O19W Sm3 89.7(19) . .
Sm4 O20W Sm4 68.5(18) 3_575 .
Sm3 O23W Sm3 67.1(18) . 3_585
Sm4 O26W Sm3 104(2) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sm1 O14 2.361(13) .
Sm1 O1A 2.363(16) .
Sm1 O29 2.367(14) .
Sm1 O24 2.398(13) .
Sm1 O9 2.421(13) .
Sm1 O32 2.428(12) .
Sm1 O1W 2.511(14) .
Sm1 O2W 2.518(14) .
Sm2 O4W 2.372(14) .
Sm2 O10 2.401(12) .
Sm2 O6W 2.402(16) .
Sm2 O8W 2.418(14) .
Sm2 O3W 2.421(14) .
Sm2 O7W 2.438(15) .
Sm2 O9W 2.441(14) .
Sm2 O5W 2.460(14) .
Sm3 O23W 2.10(7) .
Sm3 O25W 2.37(6) .
Sm3 O23W 2.39(6) 3_585
Sm3 Sm3 2.492(11) 3_585
Sm3 O21W 2.55(7) .
Sm3 O26W 2.60(7) .
Sm3 O19W 2.75(6) .
Sm3 Sm4 3.719(8) .
Sm4 O20W 2.02(6) 3_575
Sm4 O26W 2.11(7) .
Sm4 O24W 2.47(6) .
Sm4 O19W 2.51(6) .
Sm4 O20W 2.56(6) .
Sm4 Sm4 2.620(11) 3_575
Si1 O38 1.606(12) .
Si1 O39 1.612(12) .
Si1 O37 1.626(12) .
Si1 O36 1.642(13) .
W1 O1 1.744(14) .
W1 O22 1.881(12) .
W1 O31 1.913(12) .
W1 O13 1.918(12) .
W1 O23 1.926(14) .
W1 O39 2.335(11) .
W2 O2 1.731(14) .
W2 O14 1.757(13) .
W2 O18 1.931(13) .
W2 O23 1.961(12) .
W2 O35 2.050(13) .
W2 O39 2.350(12) .
W3 O3 1.707(16) .
W3 O25 1.858(14) .
W3 O35 1.888(13) .
W3 O31 1.927(12) .
W3 O20 1.932(13) .
W3 O39 2.396(12) .
W4 O4 1.714(15) .
W4 O26 1.842(12) .
W4 O34 1.917(12) .
W4 O30 1.936(12) .
W4 O25 1.945(13) .
W4 O38 2.405(11) .
W5 O5 1.713(12) .
W5 O33 1.896(13) .
W5 O19 1.912(14) .
W5 O30 1.916(12) .
W5 O17 1.920(14) .
W5 O38 2.343(11) .
W6 O6 1.703(14) .
W6 O29 1.750(14) .
W6 O18 1.880(13) .
W6 O17 1.928(15) .
W6 O26 2.045(12) .
W6 O38 2.379(12) .
W7 O7 1.742(13) .
W7 O16 1.820(12) .
W7 O19 1.892(14) .
W7 O12 1.939(13) .
W7 O28 1.961(13) .
W7 O36 2.314(12) .
W8 O8 1.717(13) .
W8 O15 1.809(11) .
W8 O22 1.934(12) .
W8 O12 1.941(13) .
W8 O21 1.984(12) .
W8 O36 2.374(12) .
W9 O9 1.751(13) 1_565
W9 O20 1.887(13) .
W9 O28 1.898(13) .
W9 O21 1.898(14) .
W9 O34 1.905(12) .
W9 O36 2.315(12) .
W10 O10 1.743(13) .
W10 O32 1.761(12) .
W10 O13 1.901(12) .
W10 O27 1.950(12) .
W10 O15 2.118(12) .
W10 O37 2.209(11) .
W11 O11 1.727(12) .
W11 O24 1.769(13) .
W11 O33 1.919(13) .
W11 O27 1.940(12) .
W11 O16 2.075(12) .
W11 O37 2.269(11) .
O9 W9 1.751(13) 1_545
S1 S1' 1.22(4) .
S1 O1A 1.494(18) .
S1 C2 1.69(3) .
S1 C1 1.70(3) .
S1' O1A 1.36(4) .
S1' C1 1.70(5) .
S1' C2 1.71(5) .
C1 H1A 0.9700 .
C1 H1B 0.9700 .
C2 H2A 0.9700 .
C2 H2B 0.9700 .
O20W Sm4 2.02(6) 3_575
O23W Sm3 2.39(6) 3_585
